Download presentation

Presentation is loading. Please wait.

Published byNikolas Hinkson Modified over 2 years ago

1
Chapter 5 - 1 ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does diffusion depend on structure and temperature? Chapter 5: Diffusion in Solids

2
Chapter 5 - 2 Diffusion Diffusion - Mass transport by atomic motion Mechanisms Gases & Liquids – random (Brownian) motion Solids – vacancy diffusion or interstitial diffusion

3
Chapter 5 - 3 Interdiffusion: In an alloy, atoms tend to migrate from regions of high conc. to regions of low conc. Initially Adapted from Figs. 5.1 and 5.2, Callister 7e. Diffusion After some time

4
Chapter 5 - 4 Self-diffusion: In an elemental solid, atoms also migrate. Label some atomsAfter some time Diffusion A B C D

5
Chapter 5 - 5 Diffusion Mechanisms Vacancy Diffusion: atoms exchange with vacancies applies to substitutional impurities atoms rate depends on: --number of vacancies --activation energy to exchange. increasing elapsed time

6
Chapter 5 - 6 Simulation of interdiffusion across an interface: Rate of substitutional diffusion depends on: --vacancy concentration --frequency of jumping. (Courtesy P.M. Anderson) Diffusion Simulation

7
Chapter 5 - 7 Diffusion Mechanisms Interstitial diffusion – smaller atoms can diffuse between atoms. More rapid than vacancy diffusion Adapted from Fig. 5.3 (b), Callister 7e.

8
Chapter 5 - 8 Adapted from chapter-opening photograph, Chapter 5, Callister 7e. (Courtesy of Surface Division, Midland-Ross.) Case Hardening: --Diffuse carbon atoms into the host iron atoms at the surface. --Example of interstitial diffusion is a case hardened gear. Result: The presence of C atoms makes iron (steel) harder. Processing Using Diffusion

9
Chapter 5 - 9 Doping silicon with phosphorus for n-type semiconductors: Process: 3. Result: Doped semiconductor regions. silicon Processing Using Diffusion magnified image of a computer chip 0.5 mm light regions: Si atoms light regions: Al atoms 2. Heat it. 1. Deposit P rich layers on surface. silicon Adapted from chapter-opening photograph, Chapter 18, Callister 7e.

10
Chapter 5 - 10 Diffusion How do we quantify the amount or rate of diffusion? Measured empirically –Make thin film (membrane) of known surface area –Impose concentration gradient –Measure how fast atoms or molecules diffuse through the membrane M = mass diffused time J slope

11
Chapter 5 - 11 Steady-State Diffusion Fick’s first law of diffusion C1C1 C2C2 x C1C1 C2C2 x1x1 x2x2 D diffusion coefficient Rate of diffusion independent of time Flux proportional to concentration gradient =

12
Chapter 5 - 12 Example: Chemical Protective Clothing (CPC) Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn. If butyl rubber gloves (0.04 cm thick) are used, what is the diffusive flux of methylene chloride through the glove? Data: –diffusion coefficient in butyl rubber: D = 110 x10 -8 cm 2 /s –surface concentrations: C 2 = 0.02 g/cm 3 C 1 = 0.44 g/cm 3

13
Chapter 5 - 13 Example (cont). glove C1C1 C2C2 skin paint remover x1x1 x2x2 Solution – assuming linear conc. gradient D = 110 x 10 -8 cm 2 /s C 2 = 0.02 g/cm 3 C 1 = 0.44 g/cm 3 x 2 – x 1 = 0.04 cm Data:

14
Chapter 5 - 14 Diffusion and Temperature Diffusion coefficient increases with increasing T. D DoDo exp QdQd RT = pre-exponential [m 2 /s] = diffusion coefficient [m 2 /s] = activation energy [J/mol or eV/atom] = gas constant [8.314 J/mol-K] = absolute temperature [K] D DoDo QdQd R T

15
Chapter 5 - 15 Diffusion and Temperature Adapted from Fig. 5.7, Callister 7e. (Date for Fig. 5.7 taken from E.A. Brandes and G.B. Brook (Ed.) Smithells Metals Reference Book, 7th ed., Butterworth-Heinemann, Oxford, 1992.) D has exponential dependence on T D interstitial >> D substitutional C in -Fe C in -Fe Al in Al Fe in -Fe Fe in -Fe 1000 K/T D (m 2 /s) C in -Fe C in -Fe Al in Al Fe in -Fe Fe in -Fe 0.51.01.5 10 -20 10 -14 10 -8 T( C) 1500 1000 600 300

16
Chapter 5 - 16 Example: At 300ºC the diffusion coefficient and activation energy for Cu in Si are D(300ºC) = 7.8 x 10 -11 m 2 /s Q d = 41.5 kJ/mol What is the diffusion coefficient at 350ºC? transform data D Temp = T ln D 1/T

17
Chapter 5 - 17 Example (cont.) T 1 = 273 + 300 = 573 K T 2 = 273 + 350 = 623 K D 2 = 15.7 x 10 -11 m 2 /s

18
Chapter 5 - 18 Non-steady State Diffusion The concentration of diffucing species is a function of both time and position C = C(x,t) In this case Fick’s Second Law is used Fick’s Second Law

19
Chapter 5 - 19 Non-steady State Diffusion Adapted from Fig. 5.5, Callister 7e. B.C. at t = 0, C = C o for 0 x at t > 0, C = C S for x = 0 (const. surf. conc.) C = C o for x = Copper diffuses into a bar of aluminum. pre-existing conc., C o of copper atoms Surface conc., C of Cu atoms bar s C s

20
Chapter 5 - 20 Solution: C(x,t) = Conc. at point x at time t erf (z) = error function erf(z) values are given in Table 5.1 CSCS CoCo C(x,t)C(x,t)

21
Chapter 5 - 21 Non-steady State Diffusion Sample Problem: An FCC iron-carbon alloy initially containing 0.20 wt% C is carburized at an elevated temperature and in an atmosphere that gives a surface carbon concentration constant at 1.0 wt%. If after 49.5 h the concentration of carbon is 0.35 wt% at a position 4.0 mm below the surface, determine the temperature at which the treatment was carried out. Solution: use Eqn. 5.5

22
Chapter 5 - 22 Solution (cont.): –t = 49.5 h x = 4 x 10 -3 m –C x = 0.35 wt%C s = 1.0 wt% –C o = 0.20 wt% erf(z) = 0.8125

23
Chapter 5 - 23 Solution (cont.): We must now determine from Table 5.1 the value of z for which the error function is 0.8125. An interpolation is necessary as follows zerf(z) 0.900.7970 z0.8125 0.950.8209 z 0.93 Now solve for D

24
Chapter 5 - 24 To solve for the temperature at which D has above value, we use a rearranged form of Equation (5.9a); from Table 5.2, for diffusion of C in FCC Fe D o = 2.3 x 10 -5 m 2 /s Q d = 148,000 J/mol Solution (cont.): T = 1300 K = 1027°C

25
Chapter 5 - 25 Example: Chemical Protective Clothing (CPC) Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn. If butyl rubber gloves (0.04 cm thick) are used, what is the breakthrough time (t b ), i.e., how long could the gloves be used before methylene chloride reaches the hand? Data (from Table 22.5) –diffusion coefficient in butyl rubber: D = 110 x10 -8 cm 2 /s

26
Chapter 5 - 26 Example (cont). Time required for breakthrough ca. 4 min glove C1C1 C2C2 skin paint remover x1x1 x2x2 Solution – assuming linear conc. gradient Equation 22.24 D = 110 x 10 -8 cm 2 /s

27
Chapter 5 - 27 Diffusion FASTER for... open crystal structures materials w/secondary bonding smaller diffusing atoms lower density materials Diffusion SLOWER for... close-packed structures materials w/covalent bonding larger diffusing atoms higher density materials Summary

28
Chapter 5 - 28 Core Problems: Self-help Problems: ANNOUNCEMENTS Reading:

Similar presentations

OK

ME 210 Exam 2 Review Session Dr. Aaron L. Adams, Assistant Professor.

ME 210 Exam 2 Review Session Dr. Aaron L. Adams, Assistant Professor.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on bluetooth based smart sensor networks definition Ppt on parallel lines Ppt on solar system for class 8th Ppt on power diode characteristics Ppt on area of parallelogram and triangles in geometry Ppt on coalition government wwi Ppt on google driverless car Convert word doc to ppt online shopping Ppt on column chromatography uses Ppt on linux shell scripting